APSe6 (A = K, Rb, and Cs): Polymeric Selenophosphates with Reversible Phase-Change Properties
In Chung; Junghwan Do; Christian G. Canlas; David P. Weliky; Mercouri G. Kanatzidis; Inorganic Chemistry 43 (2004) 2762–2764; doi:10.1021/ic035448q

data_4310931
_publ_section_title
;
 APSe6 (A = K, Rb, and Cs): Polymeric Selenophosphates with Reversible
 Phase-Change Properties
;
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              2762
_journal_page_last               2764
_journal_paper_doi               10.1021/ic035448q
_journal_volume                  43
_journal_year                    2004
_chemical_formula_sum            'P Rb Se6'
_chemical_formula_weight         590.20
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           29
_symmetry_cell_setting           orthorhombic
_symmetry_space_group_name_Hall  'P 2c -2ac'
_symmetry_space_group_name_H-M   'P c a 21'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_formula_units_Z            4
_cell_length_a                   11.7764(17)
_cell_length_b                   6.8580(10)
_cell_length_c                   11.4596(16)
_cell_measurement_temperature    293(2)
_cell_volume                     925.5(2)
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.978
_diffrn_measured_fraction_theta_max 0.978
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0470
_diffrn_reflns_av_sigmaI/netI    0.0394
_diffrn_reflns_limit_h_max       15
_diffrn_reflns_limit_h_min       -15
_diffrn_reflns_limit_k_max       9
_diffrn_reflns_limit_k_min       -8
_diffrn_reflns_limit_l_max       14
_diffrn_reflns_limit_l_min       -14
_diffrn_reflns_number            8770
_diffrn_reflns_theta_full        28.32
_diffrn_reflns_theta_max         28.32
_diffrn_reflns_theta_min         2.97
_exptl_absorpt_coefficient_mu    29.031
_exptl_crystal_density_diffrn    4.236
_exptl_crystal_density_method    'not measured'
_exptl_crystal_F_000             1024
_refine_diff_density_max         0.916
_refine_diff_density_min         -0.924
_refine_diff_density_rms         0.322
_refine_ls_abs_structure_details 'Flack H D (1983), Acta Cryst. A39, 876-881'
_refine_ls_abs_structure_Flack   0.052(19)
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   0.977
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     73
_refine_ls_number_reflns         2193
_refine_ls_number_restraints     1
_refine_ls_restrained_S_all      0.977
_refine_ls_R_factor_all          0.0351
_refine_ls_R_factor_gt           0.0259
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.0233P)^2^+0.0000P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0499
_refine_ls_wR_factor_ref         0.0523
_reflns_number_gt                1894
_reflns_number_total             2193
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ic035448qsi20031217_113002_2.cif
_cod_data_source_block           rbpse6s
_cod_database_code               4310931